Supported quantum clusters of silver as enhanced catalysts for reduction
© Leelavathi et al; licensee Springer. 2011
Received: 20 September 2010
Accepted: 8 February 2011
Published: 8 February 2011
Quantum clusters (QCs) of silver such as Ag7(H2MSA)7, Ag8(H2MSA)8 (H2MSA, mercaptosuccinic acid) were synthesized by the interfacial etching of Ag nanoparticle precursors and were loaded on metal oxide supports to prepare active catalysts. The supported clusters were characterized using high resolution transmission electron microscopy, scanning electron microscopy, X-ray photoelectron spectroscopy, and laser desorption ionization mass spectrometry. We used the conversion of nitro group to amino group as a model reaction to study the catalytic reduction activity of the QCs. Various aromatic nitro compounds, namely, 3-nitrophenol (3-np), 4-nitrophenol (4-np), 3-nitroaniline (3-na), and 4-nitroaniline (4-na) were used as substrates. Products were confirmed using UV-visible spectroscopy and electrospray ionization mass spectrometry. The supported QCs remained active and were reused several times after separation. The rate constant suggested that the reaction followed pseudo-first-order kinetics. The turn-over frequency was 1.87 s-1 per cluster for the reduction of 4-np at 35°C. Among the substrates investigated, the kinetics followed the order, SiO2 > TiO2 > Fe2O3 > Al2O3.
Monolayer-protected quantum clusters (QCs) composed of a few atoms show unique properties due to their novel atomic and electronic structure. Their discrete electronic states produce well-defined luminescence in clusters, such as Au25, Au23, Au22, Au8, etc. [1–7]. They have attracted the attention of various fields such as sensors, biolabels, live cell-targeted imaging , single molecule electroluminescence , opto-electronics , and catalysis . In the case of Au25, single crystal X-ray analysis has shown that it has an Au13 core protected with six [Au(SR)2] units in a core-shell-like pattern. The icosahedral Au13 core has 20 triangular faces. However, only 12 facets are face-capped by the exterior 12 Au atoms which keep eight facets open . These "hole" sites may be useful as active sites  which may participate in catalytic processes. Although the single crystal structures of the most of the clusters are yet to be solved, it is expected that many of them contain active sites. In this study, electron transfer properties of Ag7 and Ag8 clusters were explored using a simple reduction reaction, namely, the conversion of nitro to amino group, in different substrates. Catalysis using noble metals has caused great excitement after the initial report of Haruta . It is known that reduction potential of silver nanoparticles change with size and shifts to more negative values with decrease in size, which are in good agreement with previous predictions . QCs have very high negative reduction potential in comparison to bulk, and this makes them useful for the catalysis of electron transfer reactions. Silver is less expensive than other noble metals, and it was reported as an efficient catalyst for several reactions. For example, silver on alumina is a promising catalyst for selective catalytic reduction of NO by hydrocarbons from automobile exhausts . It has been reported that Ag nanoparticles on hydroxyapatite in the presence of water catalyze the selective oxidation of various phenylsilanes into phenylsilanols  and also that the same system was found to be a highly efficient catalyst for the selective hydration of nitriles to amides . It has been reported that chloroanilines were produced in large scale by the hydrogenation of chloronitrobenzenes using Ag nanoparticles on SiO2, and the system also showed the size-dependent catalytic activity . Formation of subsurface oxygen on the catalyst, enhanced in the case of supported silver clusters, plays an important role in CO oxidation . Ag clusters supported on alumina are better active when compared to platinum supported on alumina for oxidant-free alcohol dehydrogenation to carbonyl compounds, and clusters less than 1 nm show structure-sensitive reactions . It is reported that alumina is the best support for Ag, and it shows better selectivity for oxidation of ammonia to form nitrogen at low temperatures . Silver nanoclusters on TiO2 enhance the reduction of bis (2-dipyridyl) disulfide to 2-mercaptopyridine in the presence of water . It has been reported that the selectivity for hydrogenation of crotonaldehyde was very high in the presence of Ag catalyst below 3-nm diameter; the catalyst was also structure sensitive . Shimizu et al.  reported that clusters of silver on alumina catalyze the cross-coupling reactions of alcohols, direct amide synthesis from alcohols and amines , and chemoselective reduction of a nitrostyrene with size-dependent catalytic activity . The highest yield was obtained with particles of size ranging from 0.9 to 30 nm for the N-alkylation of anilines with benzyl alcohol for which silver shows high selectivity compared to other catalysts due to less stable metal-hydride bond formation . Several reports are available for the reduction of nitro groups using nanoparticles [27–32]. Pal et al. reported the reduction of 4-nitrophenol (4-np) using silver nanoshells stabilized with cationic polystyrene beads  as well as silver deposited on silica gel . It was reported that gold nanoparticles containing membranes reduce aromatic nitro compounds . Ag and Au nanoparticles grown on calcium alginate gel beads are found to catalyze nitrophenol reduction .
In this article, we studied the catalysis of supported QCs of Ag7,8 using 4-np as the model system. Ag7 and Ag8 are new QCs prepared efficiently by the interfacial method . Similar silver clusters are also made by other routes . The reduction reaction occurs with a rate constant of 8.23 × 10-3 at 35°C, and the TOF measured was 1.87 s-1 per cluster. Performance of various supports has been evaluated.
All the following chemicals were commercially available and were used without further purification. Silver nitrate (AgNO3, 99%), mercaptosuccinic acid (MSA, 97%), methanol (GR grade), toluene (GR grade), and alumina were purchased from SRL Chemical Co. Ltd., India Mumbai. Trisodium citrate (Qualigens) Mumbai, India, titanium dioxide (Ranbaxy Fine Chemicals Limited) Mumbai, India, silica (Sisco Research Laboratories Private Limited) Mumbai, India, and iron oxide (Merck Specialties Private Limited) Mumbai, India were purchased from the mentioned laboratories. Sodium borohydride (NaBH4, 98%) was purchased from Sigma Aldrich. 4-np (C6H5NO3, 97%) and 4-aminophenol (C6H7NO, 98%) were purchased from Loba Chemicals. 3-np (C6H5NO3, 97%), 3-na (C6H6N2O2, 98%) and 4-na (C6H6N2O2, 98%) were purchased from SD fine chemicals.
Preparation of Ag@MSA nanoparticles
Mercaptosuccinic acid-capped silver nanoparticles were synthesized according to the reported method . MSA (1795 mg) was dissolved in methanol (400 ml) and the mixture was kept under vigorous stirring in an ice bath. A solution of silver nitrate (340 mg) in 6.792 ml water was added. A freshly prepared aqueous solution of sodium borohydride (756.6 mg in 100 ml of water) was added drop by drop. The colorless solution changed to yellow, and further addition of NaBH4 changed it to brown. The solution was kept for half an hour for stirring. The particles were allowed to settle down in methanol, which were filtered and washed with methanol. The sample was again dispersed in methanol and centrifuged to remove excess thiols attached on the surface of the particles. The solvent was removed by rotavapor, in order to get a powder. These particles were freely dispersible in water. The UV-vis absorption spectrum shows a plasmon absorption around 390 nm for the as-prepared metallic Ag@MSA nanoparticles.
Preparation of Ag QCs
Silver QCs were prepared by the interfacial etching method as per our earlier article . In brief, 100 ml of toluene was added to the MSA solution (MSA 300 mg/100 ml of toluene/75 ml of water). This forms two phases, and the mixture was kept under vigorous stirring. To this, 100 mg of Ag@MSA nanoparticles in 25 ml of water was added (nanoparticles and MSA were in 1:3 ratio by mass). The etching process took place at the interface of the two phases (water/toluene). The color of the aqueous phase changed to yellow from dark brown. After 48 h of continuous stirring, it changed to orange. In the UV-vis absorption spectrum, the plasmon peak disappeared, which shows that no metallic behavior was retained in Ag QCs, and a new peak around 550 nm appeared due to intra-band transitions. The formed QCs were dissolved in the aqueous phase and were separated by freeze drying to obtain a powder. Mixture of dried QCs had an Ag8:Ag7 ratio of 80:20 . Although they were separated in the earlier article , the mixture was used directly in this study in view of the quantities needed.
Ag QCs supported on alumina
Alumina powder (60-325 mesh BSS) was added to aqueous Ag8,7 QC solutions, and the mixture was stirred for 5 min. Color of the alumina powder changed to orange, indicating that the QCs of Ag7,8 got loaded on alumina. The intensity of the color in the solution decreased, and finally, the solution became colorless. The amount of QCs in the solution was controlled to get various weight ratios of loading. The QC loaded materials were washed with water and dried in ambient air. Maximum loading corresponded to 0.1/1 g.
Preparation of Ag@citrate nanoparticles
The Ag@citrate nanoparticles were prepared according to a previously published procedure . They were loaded on alumina (10% loading), as in the case of QCs.
For the reduction reaction, 1 ml of freshly prepared ice-cold aqueous solution of NaBH4 (160 mM) was introduced to 1 ml of aqueous 4-np solution (7 mM), taken in a sample bottle. Next, Al2O3@Ag7,8 (10% loading, 50 mg) was added to the above solution mixture, and time-dependent absorption spectra were measured. From changes in the absorption of 4-nitrophenolate ion at 400 nm as a function of time, the rate constants were calculated. The product was identified by comparing with the spectrum of an authentic sample of 4-aminophenol (4-ap). The experiment was carried out at 15, 25, and 35°C.
UV-vis optical absorption spectra were recorded with a Perkin-Elmer Lambda 25 instrument. Fluorescence spectroscopy measurements were carried out using a HORIBA JOBIN VYON Nano Log instrument. XPS spectra were recorded using an Omicron ESCA Probe spectrometer with unmonochromatized Mg Kα X-rays (hυ = 1253.6 eV). The samples were spotted as drop cast films on a sample stub. HRTEM of QCs coated on alumina was carried out using a JEOL 3010 instrument. The samples were cast on carbon-coated grids, and dried under ambient conditions. Scanning electron microscopy (SEM) and EDAX measurements were performed using a HITACHI S-4800 FESEM, and the samples were spotted on indium tin oxide (ITO) glass plates, followed by drying under ambient conditions. ESI-MS measurements were performed using a MDX Sciex 3200 Q-TRAP LC/MS/MS (Applied Biosystems) DST Unit of Nanoscience, IITM in which the spray and extraction are orthogonal to each other. Product formed was made to 10 ppm (1:1 ratio of water and methanol) and sprayed at 5 kV. LDI-MS studies were conducted using a Voyager DE PRO Biospectrometry Workstation of Applied Biosystems MALDI-TOF MS. A pulsed nitrogen laser of 337 nm was used for the studies.
Results and discussion
Polyacrylamide gel electrophoresis of the as-prepared clusters showed two bands. This indicated the presence of two clusters, Ag7 and Ag8 in the crude solution, which were separated and dissolved in water . The solutions exhibited strong emission. Except for these purified clusters, the excitation and emission are different from the crude clusters without separation (shown in the inset of Figure 1a). The clusters have the molecular formulae, Ag8MSA8 and Ag7MSA7, but are described merely as Ag8 and Ag7. The crude cluster is a 80:20 mixture of Ag8 and Ag7 which were used for this study. Therefore, we refer to the clusters as Ag7,8.
Additional file 1, Figure S1A shows the HRTEM image of the QCs supported on alumina. It was observed that silver QCs were uniformly coated on alumina. They were highly sensitive to the electron beam, and started to fuse and became nanoparticles upon continuous exposure. The lattice fringes with an interplanar spacing of 2.4 Å correspond to Ag (111) (Figure S1B in Additional file 1), indicating the formation of nanoparticles. Corresponding EDAX shows the presence of silver on alumina, as shown in Additional file 1, Figure S1C-E.
With the addition of QCs supported on alumina, fading and ultimate leaching of the dark yellow color due to phenolate ions occurred, and brown color of 4-ap appeared. 4-nitrophenolate ion peak at 400 nm got reduced and within 10 min, a new peak around 295 nm appeared due to 4-ap [42, 43]. The spectrum of 4-ap was verified with that of a standard sample. Reduction can be visualized with the color change, and it was almost complete which was authenticated by the optical absorbance value of 4-ap. Excess amount of reductant NaBH4 was used, and therefore, a pseudo-first-order rate equation may be considered. As a result of adsorption of 4-np and BH4 - on the cluster surface, electron transfer from donor BH4 - to the acceptor 4-nitrophenolate ion is facilitated. The reduction was carried out at three different temperatures; 15, 25, and 35°C (Figure 4a,b,c). It was observed that at lower temperatures, the time required was high. Isobestic point observed during the transformation is shown in Additional file 2, Figure S2.
The plot of ln(k) versus 1/T (Figure 5b) yields a straight line. The activation energy was found to be 55.6 kJ mol-1 at 298 K. The TOF was 1.87 s-1 per cluster. Although the calculated TOF is comparable to that reported for Ag nanoparticles (which is 1-2) , we note that certain number of atoms of the clusters are not accessible in the catalytic process as they are used for surface binding. This aspect reduces the available number of surface atoms and increases the TOF per cluster.
Catalysts remain active at the end of the reaction, and these were separated from the product. Again, a fresh batch of 4-np was added to the used catalyst. Fresh reducing agent was not needed till the completion of four cycles, but subsequent cycles required fresh BH4 -. The reaction followed the same kinetics as mentioned above. In this way, four consecutive fresh batches of 4-np were reduced with the same batch of catalyst. Reusability of the same batch of catalyst for the reduction cycles was tested; it remained active for ten cycles. The data for the second, third, fourth, and fifth reduction cycles are shown in Additional file 5, Figure S4. The product obtained was characterized with positive ion ESI-MS as shown in Additional file 6, Figure S5. Formation of 4-ap was confirmed with a peak at m/z 109, and the precursor 4-np peak at m/z 139 also got disappeared. Although the 4-np peak due to protonated 4-np (m/z 110) was not detected (which is the major peak in the pure sample), the molecular ion (m/z 109) is seen in the product. The peak at m/z 109 in the parent compound, 4-np, is due to the loss of NO . This peak in the product spectrum is not due to the presence of unreacted substrate 4-np as its molecular ion signature at m/z 139 disappeared completely.
The same experiment was performed with Ag7,8 QCs (0.5 mg/0.5 ml) alone (unsupported) in the presence of NaBH4, and complete reduction happened within 3 min. The same reduction reaction was repeated with Ag@citrate nanoparticles of 40 nm core diameter supported on alumina. For the supported Ag@citrate nanoparticles (10% loading, 50 mg), the reduction time increased thrice when compared to QCs. It appears that the electron transfer reaction depends upon the surface area of the catalyst, besides the electronic effect. This follows pseudo-first-order kinetics as shown in Additional file 8, Figure S7. The reduction time was reduced with the QCs compared with the nanoparticles.
Other nitro compounds such as 3-na, 4-na, and 3-np were tested with supported QCs (Additional file 9, Figure S8). The peaks at 225 and 358 nm indicate the progress of the reduction of 3-na. The reduction in the peak at 380 nm of 4-na indicates the progress in the reduction with the appearance of the new peaks at 240 and 305 nm. The peaks at 330 and 270 nm reduced with the appearance of the peak at 290 nm during the reduction 3-np.
Support effect in the catalysis of Ag7,8
The same experiment was performed with SiO2@Ag7,8, TiO2@Ag7,8 and Fe2O3@Ag7,8 in the presence of NaBH4. All the catalyst samples had similar Ag7,8 loading (10%). Complete reduction of 4-np happened in 1, 4 and 9 min, and their rate constant values were 1.547 × 10-1 s-1, 2.94 × 10-2 s-1, and 8.88 × 10-3 s-1 for SiO2@Ag7,8, TiO2@Ag7,8, and Fe2O3@Ag7,8, respectively. After the reaction, the catalysts were separated and reused, and the data are shown in Additional file 10, Figure S9. The order of efficiency of the catalyst, in the reduction of 4-np, is SiO2@Ag7,8 > TiO2@Ag7,8 > Fe2O3 @Ag7,8 > Al2O3@Ag7,8.
QCs, Ag7, and Ag8 were supported on various substrates to prepare catalysts, such as Al2O3@Ag7,8, SiO2@Ag7,8, TiO2@Ag7,8, and Fe2O3@Ag7,8. Such catalysts show enhanced catalytic activity for the reduction of several nitro compounds. Detailed studies were performed with Al2O3@Ag7,8. The pseudo-first-order rate constant was found to be twice larger than the supported silver of 3.29% loading on an anion exchange resin . The rate constant was found to be 8.23 × 10-3 s-1, and the activation energy was 55.6 kJ mol-1 at 298 K. Other nitro aromatics such as 3-np, 3-na, and 4-na were also investigated. The results suggest that the cluster system is a better catalyst for the reactions investigated.
Appendix: Supplementary data
HRTEM-EDAX spectrum and images of Al2O3@Ag7,8, isobestic point in the UV-vis spectra of the reduction of 4-np, increase in concentration of 4-ap during 4-np reduction reaction with corresponding plot of ln(k) versus 1/T, reusability of the supported Al2O3@Ag7,8 for the reduction of 4-np, positive ion ESI-MS of the product, XPS survey spectra of Al2O3@Ag7,8 after reactions (first and third cycles), UV-vis spectra of the reduction reaction using Ag@citrate nanoparticles with corresponding plot of concentration versus time, variation of the spectral intensities of other nitro aromatics during reduction and UV-vis spectra for the reduction of 4-np with SiO2@Ag7,8, TiO2@Ag7,8 and Fe2O3 @Ag7,8. Supplementary data pertaining to with this article can be found, in the online version, in Additional files 1, 2, 3, 4, 5, 6, 7, 8, 9 and 10.
indium tin oxide
scanning electron microscopy.
We thank the department of Science and Technology (DST), Government of India for constantly supporting our research program on nanomaterials.
- Heaven MW, Dass A, White PS, Holt KM, Murray RW: Crystal structure of the gold nanoparticle [N(C 8 H 17 ) 4 ][Au 25 (SCH 2 CH 2 Ph) 18 ]. J Am Chem Soc 2008, 130: 3754. 10.1021/ja800561bView Article
- Zheng J, Nicovich PR, Dickson RM: Highly Fluorescent Noble-Metal Quantum Dots. Ann Rev Phys Chem 2007, 58: 409. 10.1146/annurev.physchem.58.032806.104546View Article
- Zhu M, Lanni E, Garg NME, Bier ME, Jin R: Kinetically Controlled, High-Yield Synthesis of Au 25 Clusters. J Am Chem Soc 2008, 130: 1138. 10.1021/ja0782448View Article
- Habeeb Muhammed MA, Verma PK, Pal SK, Kumar ARC, Paul S, Omkumar RV, Pradeep T: Bright, NIR Emitting Au 23 from Au 25 -Characterization and Applications Including Bio-labeling. Chem Eur J 2009, 15: 10110. 10.1002/chem.200901425View Article
- Shibu ES, Radha B, Verma PK, Bhyrappa P, Kulkarni GU, Pal SK, Pradeep T: Functionalized Au 22 clusters: Synthesis characterization and patterning. ACS Appl Mater Interfaces 2009, 1: 2199. 10.1021/am900350rView Article
- Sevillano P, Fuhr O, Hampe O, Lebedkin S, Matern E, Fenske D, Kappes MM: Synthesis, Characterization, and X-ray Structure Determination of [Au 18 (P) 2 (PPh) 4 (PHPh)(dppm) 6 ]Cl 3, . Inorg Chem 2007, 46: 7294. 10.1021/ic062107eView Article
- Zheng J, Petty JT, Dickson RM: High Quantum Yield Blue Emission from Water-Soluble Au 8 Nanodots. J Am Chem Soc 2003, 125: 7780. 10.1021/ja035473vView Article
- Gonzalez JI, Vosch T, Dickson RM: Charge Injection into Discrete States of Individual Electroluminescent Au Nanoclusters. Phys Rev B 2006, 74: 235404. 10.1103/PhysRevB.74.235404View Article
- Lee TH, Gonzalez JI, Zheng J, Dickson RM: Single molecule optoelectronics. Acc Chem Res 2005, 38: 534. 10.1021/ar040146tView Article
- Haruta M: Catalysis: Gold rush. Nature 2005, 437: 1098. 10.1038/4371098aView Article
- Zhu Y, Qian H, Drake BA, Jin R: Atomically Precise Au 25 (SR) 18 Nanoparticles as Catalysts for Selective Hydrogenation of α, β-Unsaturated Ketones and Aldehydes. Angew Chem Int Ed 2010, 49: 1295. 10.1002/anie.200906249View Article
- Haruta M, Yamada N, Kobayashi T, Iijima S: Gold catalysts prepared by coprecipitation for low-temperature oxidation of hydrogen and of carbon monoxide. J Catal 1989, 115: 301. 10.1016/0021-9517(89)90034-1View Article
- Chaki NK, Sharma J, Mandle AB, Mulla IS, Pasricha R, Vijayamohanan K: Size dependent redox behavior of monolayer protected silver nanoparticles (2–7 nm) in aqueous medium. Phys Chem Chem Phys 2004, 6: 1304. 10.1039/b312643aView Article
- Shimizu KI, Satsuma A: Selective catalytic reduction of NO over supported silver catalysts--practical and mechanistic aspects. Phys Chem Chem Phys 2006, 8: 2677. 10.1039/b601794kView Article
- Mitsudome T, Arita S, Mori H, Mizugaki T, Jitsukawa K, Kaneda K: Supported Silver-Nanoparticle-Catalyzed Highly Efficient Aqueous Oxidation of Phenylsilanes to Silanols. Angew Chem Int Ed 2008, 47: 7938. 10.1002/anie.200802761View Article
- Mitsudome T, Mikami Y, Mori H, Arita S, Mizugaki T, Jitsukawa K, Kaneda K: Supported silver nanoparticle catalyst for selective hydration of nitriles to amides in water. Chem Commun 2009, 3258. 10.1039/b902469g
- Chen Y, Wang C, Liu H, Qiu J, Bao X: Ag/SiO 2 : a novel catalyst with high activity and selectivity for hydrogenation of chloronitrobenzenes. Chem Commun 2005, 5298. 10.1039/b509595f
- Qu Z, Cheng M, Huang W, Bao X: Formation of subsurface oxygen species and its high activity toward CO oxidation over silver catalysts. J Catal 2005, 229: 446. 10.1016/j.jcat.2004.11.043View Article
- Shimizu KI, Sugino K, Sawabe K, Satsuma A: Oxidant-Free Dehydrogenation of Alcohols Heterogeneously Catalyzed by Cooperation of Silver Clusters and Acid-Base Sites on Alumina. Chem Eur J 2009, 15: 2341. 10.1002/chem.200802222View Article
- Gang L, Anderson BG, van Grondelle J, van Santen RA: Low temperature selective oxidation of ammonia to nitrogen on silver-based catalysts. Appl Catal B 2003, 40: 101. 10.1016/S0926-3373(02)00129-7View Article
- Tada H, Teranishi K, Inubushi YI, Ito S: Ag Nanocluster Loading Effect on TiO 2 Photocatalytic Reduction of Bis(2-dipyridyl)disulfide to 2-Mercaptopyridine by H 2 O. Langmuir 2000, 16: 3304. 10.1021/la991315zView Article
- Claus P, Hofmeister H: Electron Microscopy and Catalytic Study of Silver Catalysts: Structure Sensitivity of the Hydrogenation of Crotonaldehyde. J Phys Chem B 1999, 103: 2766. 10.1021/jp983857fView Article
- Shimizu KI, Sato R, Satsuma A: Direct C_C Cross-Coupling of Secondary and Primary Alcohols Catalyzed by a γ-Alumina-Supported Silver Subnanocluster. Angew Chem Int Ed 2009, 48: 3982. 10.1002/anie.200901057View Article
- Shimizu KI, Ohshima K, Satsuma A: Direct Dehydrogenative Amide Synthesis from Alcohols and Amines Catalyzed by γ-Alumina Supported Silver Cluster. Chem Eur J 2009, 15: 9977. 10.1002/chem.200901896View Article
- Shimizu KI, Miyamoto Y, Satsuma A: Size- and support-dependent silver cluster catalysis for chemoselective hydrogenation of nitroaromatics. J Catal 2010, 270: 86. 10.1016/j.jcat.2009.12.009View Article
- Shimizu KI, Nishimura M, Satsuma A: γ-Alumina-Supported Silver Cluster for N -Benzylation of Anilines with Alcohols. ChemCatChem 2009, 1: 497. 10.1002/cctc.200900209View Article
- Jana S, Ghosh SK, Nath S, Pande S, Praharaj S, Panigrahi S, Basu S, Endo T, Pal T: Synthesis of silver nanoshell-coated cationic polystyrene beads: A solid phase catalyst for the reduction of 4-nitrophenol. Appl Catal A 2006, 313: 41. 10.1016/j.apcata.2006.07.007View Article
- Kundu S, Mandal M, Ghosh SK, Pal T: Photochemical deposition of SERS active silver nanoparticles on silica gel and their application as catalysts for the reduction of aromatic nitro compounds. J Colloid Interface Sci 2004, 272: 134. 10.1016/j.jcis.2003.11.046View Article
- Dotzauer DM, Bhattacharjee S, Wen Y, Bruening ML: Nanoparticle-containing membranes for the catalytic reduction of nitroaromatic compounds. Langmuir 2009, 25: 1865. 10.1021/la803220zView Article
- Kuroda K, Ishida T, Haruta M: Reduction of 4-nitrophenol to 4-aminophenol over Au nanoparticles deposited on PMMA. J Mol Catal A 2009, 298: 7. 10.1016/j.molcata.2008.09.009View Article
- Esumi K, Isono R, Yoshimura T: Preparation of PAMAM- and PPI-Metal (Silver, Platinum, and Palladium) Nanocomposites and Their Catalytic Activities for Reduction of 4-Nitrophenol. Langmuir 2004, 20: 237. 10.1021/la035440tView Article
- Mori K, Kumami A, Tomonari M, Yamashita H: A pH-Induced Size Controlled Deposition of Colloidal Ag Nanoparticles on Alumina Support for Catalytic Application. J Phys Chem C 2009, 113: 16850. 10.1021/jp907277gView Article
- Saha S, Pal A, Kundu S, Basu S, Pal T: Photochemical Green Synthesis of Calcium-Alginate-Stabilized Ag and Au Nanoparticles and Their Catalytic Application to 4-Nitrophenol Reduction. Langmuir 2010, 26: 2885. 10.1021/la902950xView Article
- Rao TUB, Pradeep T: Luminescent Ag 7 and Ag 8 Clusters by Interfacial Synthesis. Angew Chem Int Ed 2010, 49: 3925. 10.1002/anie.201000527View Article
- Diez I, Pusa M, Kulmala S, Jiang H, Walther A, Goldmann AS, Muller AHE, Ikkala O, Ras RHA: Color Tunability and Electrochemiluminescence of Silver Nanoclusters. Angew Chem Int Ed 2009, 121: 2156.View Article
- Kimura K, Yao H, Sato S: Self-assembling of gold and silver nanoparticles at a hydrophilic/hydrophobic interface: A synthetic aspect and superstructure formation. Synth React Inorg Met Org Nano Met Chem 2006, 36: 237.View Article
- Bootharaju MS, Pradeep T: Uptake of toxic metal ions from water by naked and monolayer protected silver nanoparticles: An X-ray photoelectron spectroscopic investigation. J Phys Chem C 2010, 114: 8328. 10.1021/jp101988hView Article
- Mrudula KV, Rao TUB, Pradeep T: Interfacial synthesis of luminescent 7 kDa silver clusters. J Mater Chem 2009, 19: 4335. 10.1039/b900025aView Article
- Wu Z, Lanni E, Chen W, Bier ME, Ly D, Jin R: High Yield, Large Scale Synthesis of Thiolate-Protected Ag 7 Clusters. J Am Chem Soc 2009, 131: 16672. 10.1021/ja907627fView Article
- Praharaj S, Nath S, Ghosh SK, Kundu S, Pal T: Immobilization and Recovery of Au Nanoparticles from Anion Exchange Resin: Resin-Bound Nanoparticle Matrix as a Catalyst for the Reduction of 4-Nitrophenol. Langmuir 2004, 20: 9889. 10.1021/la0486281View Article
- Sharma NC, Sahi SV, Nath S, Parsons JG, Torresdey JL-G, Pal T: Synthesis of Plant-Mediated Gold Nanoparticles and Catalytic Role of Biomatrix-Embedded Nanomaterials. Environ Sci Technol 2007, 41: 5137. 10.1021/es062929aView Article
- Oh SD, Kim MR, Choi SH, Chun JH, Lee KP, Gopalan A, Hwang CG, Sang-Ho K, Hoon OJ: Radiolytic synthesis of Pd-M (M = Ag, Au, Cu, Ni and Pt) alloy nanoparticles and their use in reduction of 4-nitrophenol. J Ind Eng Chem 2008, 14: 687.View Article
- Pradhan N, Pal A, Pal T: Silver Nanoparticle Catalyzed Reduction of Aromatic Nitro Compounds. Colloids Surf A 2002, 196: 247. 10.1016/S0927-7757(01)01040-8View Article
- Rahman-Setayesh S, Arshadi MR: Positive and negative ions mass spectra of ring substituted nitrobenzenes. J Sci I R Iran 1993, 4: 290.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.